LMucko/crystallography-open-database huggingface dataset:
Pressure-induced phase transitions in AgCl, AgBr, and AgI Sample: P = 14.3 GPa, Phase V
Hull, S.; Keen, D. A.; Physical Review B 59 (1999) 750–761; doi:10.1103/PhysRevB.59.750

data_9011702
_publ_section_title
;
 Pressure-induced phase transitions in AgCl, AgBr, and AgI
 Sample: P = 14.3 GPa, Phase V
;
_journal_name_full               'Physical Review B'
_journal_page_first              750
_journal_page_last               761
_journal_paper_doi               10.1103/PhysRevB.59.750
_journal_volume                  59
_journal_year                    1999
_chemical_formula_structural     AgI
_chemical_formula_sum            'Ag I'
_space_group_IT_number           4
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.39
_cell_angle_gamma                90
_cell_length_a                   4.007
_cell_length_b                   4.064
_cell_length_c                   5.546
_cell_formula_units_Z            2
_cell_volume                     88.833
_database_code_amcsd             0015233
_diffrn_ambient_pressure         1.43e+07
_exptl_crystal_density_diffrn    8.777
_cod_database_code               9011702
_amcsd_formula_title             AgI
Pressure-induced phase transitions in AgCl, AgBr, and AgI Sample: P = 14.5 GPa, Phase V
Hull, S.; Keen, D. A.; Physical Review B 59 (1999) 750–761; doi:10.1103/PhysRevB.59.750

data_9011703
_publ_section_title
;
 Pressure-induced phase transitions in AgCl, AgBr, and AgI
 Sample: P = 14.5 GPa, Phase V
;
_journal_name_full               'Physical Review B'
_journal_page_first              750
_journal_page_last               761
_journal_paper_doi               10.1103/PhysRevB.59.750
_journal_volume                  59
_journal_year                    1999
_chemical_formula_structural     AgI
_chemical_formula_sum            'Ag I'
_space_group_IT_number           4
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.55
_cell_angle_gamma                90
_cell_length_a                   4.001
_cell_length_b                   4.067
_cell_length_c                   5.545
_cell_formula_units_Z            2
_cell_volume                     88.703
_database_code_amcsd             0015234
_diffrn_ambient_pressure         1.45e+07
_exptl_crystal_density_diffrn    8.790
_cod_database_code               9011703
_amcsd_formula_title             AgI
Location of deuterium in alpha-scandium
Saw, C. K.; Beaudry, B. J.; Stassis, C.; Physical Review B - Condensed Matter 27 (1983) 7013–7017; doi:10.1103/PhysRevB.27.7013

data_9011704
_publ_section_title
;
 Location of deuterium in alpha-scandium
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              7013
_journal_page_last               7017
_journal_paper_doi               10.1103/PhysRevB.27.7013
_journal_volume                  27
_journal_year                    1983
_chemical_compound_source        Synthetic
_chemical_formula_sum            Sc
_chemical_name_common            Scandium
_chemical_name_mineral           Scandium
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   3.3088
_cell_length_b                   3.3088
_cell_length_c                   5.2680
_cell_formula_units_Z            2
_cell_volume                     49.948
_database_code_amcsd             0015237
_exptl_crystal_density_diffrn    2.989
_cod_database_code               9011704
X-ray diffraction and equation of state of solid neon to 110 GPa Sample: at T = 300 K and P = 10 GPa
Hemley, R. J.; Zha, C. S.; Jephcoat, A. P.; Mao, H. K.; Finger, L. W.; Cox, D. E.; Physical Review B - Condensed Matter 39 (1989) 11820–11827; doi:10.1103/PhysRevB.39.11820

data_9011705
_publ_section_title
;
 X-ray diffraction and equation of state of solid neon to 110 GPa
 Sample: at T = 300 K and P = 10 GPa
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              11820
_journal_page_last               11827
_journal_paper_doi               10.1103/PhysRevB.39.11820
_journal_volume                  39
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ne
_chemical_name_common            Neon
_chemical_name_mineral           Neon
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_formula_units_Z            4
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.567
_cell_length_b                   3.567
_cell_length_c                   3.567
_cell_volume                     45.385
_database_code_amcsd             0015239
_diffrn_ambient_pressure         1e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    2.953
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9011705
X-ray diffraction and equation of state of solid neon to 110 GPa Sample: at T = 300 K and P = 20 GPa
Hemley, R. J.; Zha, C. S.; Jephcoat, A. P.; Mao, H. K.; Finger, L. W.; Cox, D. E.; Physical Review B - Condensed Matter 39 (1989) 11820–11827; doi:10.1103/PhysRevB.39.11820

data_9011706
_publ_section_title
;
 X-ray diffraction and equation of state of solid neon to 110 GPa
 Sample: at T = 300 K and P = 20 GPa
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              11820
_journal_page_last               11827
_journal_paper_doi               10.1103/PhysRevB.39.11820
_journal_volume                  39
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ne
_chemical_name_common            Neon
_chemical_name_mineral           Neon
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_formula_units_Z            4
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.400
_cell_length_b                   3.400
_cell_length_c                   3.400
_cell_volume                     39.304
_database_code_amcsd             0015240
_diffrn_ambient_pressure         2e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    3.410
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9011706
X-ray diffraction and equation of state of solid neon to 110 GPa Sample: at T = 300 K and P = 27.1 GPa
Hemley, R. J.; Zha, C. S.; Jephcoat, A. P.; Mao, H. K.; Finger, L. W.; Cox, D. E.; Physical Review B - Condensed Matter 39 (1989) 11820–11827; doi:10.1103/PhysRevB.39.11820

data_9011707
_publ_section_title
;
 X-ray diffraction and equation of state of solid neon to 110 GPa
 Sample: at T = 300 K and P = 27.1 GPa
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              11820
_journal_page_last               11827
_journal_paper_doi               10.1103/PhysRevB.39.11820
_journal_volume                  39
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ne
_chemical_name_common            Neon
_chemical_name_mineral           Neon
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_formula_units_Z            4
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.315
_cell_length_b                   3.315
_cell_length_c                   3.315
_cell_volume                     36.429
_database_code_amcsd             0015241
_diffrn_ambient_pressure         2.71e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    3.679
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9011707
X-ray diffraction and equation of state of solid neon to 110 GPa Sample: at T = 300 K and P = 31 GPa
Hemley, R. J.; Zha, C. S.; Jephcoat, A. P.; Mao, H. K.; Finger, L. W.; Cox, D. E.; Physical Review B - Condensed Matter 39 (1989) 11820–11827; doi:10.1103/PhysRevB.39.11820

data_9011708
_publ_section_title
;
 X-ray diffraction and equation of state of solid neon to 110 GPa
 Sample: at T = 300 K and P = 31 GPa
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              11820
_journal_page_last               11827
_journal_paper_doi               10.1103/PhysRevB.39.11820
_journal_volume                  39
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ne
_chemical_name_common            Neon
_chemical_name_mineral           Neon
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_formula_units_Z            4
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.258
_cell_length_b                   3.258
_cell_length_c                   3.258
_cell_volume                     34.582
_database_code_amcsd             0015242
_diffrn_ambient_pressure         3.1e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    3.876
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9011708
X-ray diffraction and equation of state of solid neon to 110 GPa Sample: at T = 300 K and P = 35.6 GPa
Hemley, R. J.; Zha, C. S.; Jephcoat, A. P.; Mao, H. K.; Finger, L. W.; Cox, D. E.; Physical Review B - Condensed Matter 39 (1989) 11820–11827; doi:10.1103/PhysRevB.39.11820

data_9011709
_publ_section_title
;
 X-ray diffraction and equation of state of solid neon to 110 GPa
 Sample: at T = 300 K and P = 35.6 GPa
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              11820
_journal_page_last               11827
_journal_paper_doi               10.1103/PhysRevB.39.11820
_journal_volume                  39
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ne
_chemical_name_common            Neon
_chemical_name_mineral           Neon
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_formula_units_Z            4
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.230
_cell_length_b                   3.230
_cell_length_c                   3.230
_cell_volume                     33.698
_database_code_amcsd             0015243
_diffrn_ambient_pressure         3.56e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    3.978
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9011709
X-ray diffraction and equation of state of solid neon to 110 GPa Sample: at T = 300 K and P = 40.3 GPa
Hemley, R. J.; Zha, C. S.; Jephcoat, A. P.; Mao, H. K.; Finger, L. W.; Cox, D. E.; Physical Review B - Condensed Matter 39 (1989) 11820–11827; doi:10.1103/PhysRevB.39.11820

data_9011710
_publ_section_title
;
 X-ray diffraction and equation of state of solid neon to 110 GPa
 Sample: at T = 300 K and P = 40.3 GPa
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              11820
_journal_page_last               11827
_journal_paper_doi               10.1103/PhysRevB.39.11820
_journal_volume                  39
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ne
_chemical_name_common            Neon
_chemical_name_mineral           Neon
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_formula_units_Z            4
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.190
_cell_length_b                   3.190
_cell_length_c                   3.190
_cell_volume                     32.462
_database_code_amcsd             0015244
_diffrn_ambient_pressure         4.03e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.129
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9011710
X-ray diffraction and equation of state of solid neon to 110 GPa Sample: at T = 300 K and P = 51.5 GPa
Hemley, R. J.; Zha, C. S.; Jephcoat, A. P.; Mao, H. K.; Finger, L. W.; Cox, D. E.; Physical Review B - Condensed Matter 39 (1989) 11820–11827; doi:10.1103/PhysRevB.39.11820

data_9011711
_publ_section_title
;
 X-ray diffraction and equation of state of solid neon to 110 GPa
 Sample: at T = 300 K and P = 51.5 GPa
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              11820
_journal_page_last               11827
_journal_paper_doi               10.1103/PhysRevB.39.11820
_journal_volume                  39
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ne
_chemical_name_common            Neon
_chemical_name_mineral           Neon
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_formula_units_Z            4
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.139
_cell_length_b                   3.139
_cell_length_c                   3.139
_cell_volume                     30.930
_database_code_amcsd             0015245
_diffrn_ambient_pressure         5.15e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.334
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9011711
X-ray diffraction and equation of state of solid neon to 110 GPa Sample: at T = 300 K and P = 56.9 GPa
Hemley, R. J.; Zha, C. S.; Jephcoat, A. P.; Mao, H. K.; Finger, L. W.; Cox, D. E.; Physical Review B - Condensed Matter 39 (1989) 11820–11827; doi:10.1103/PhysRevB.39.11820

data_9011712
_publ_section_title
;
 X-ray diffraction and equation of state of solid neon to 110 GPa
 Sample: at T = 300 K and P = 56.9 GPa
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              11820
_journal_page_last               11827
_journal_paper_doi               10.1103/PhysRevB.39.11820
_journal_volume                  39
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ne
_chemical_name_common            Neon
_chemical_name_mineral           Neon
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_formula_units_Z            4
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.111
_cell_length_b                   3.111
_cell_length_c                   3.111
_cell_volume                     30.109
_database_code_amcsd             0015246
_diffrn_ambient_pressure         5.69e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.452
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9011712
X-ray diffraction and equation of state of solid neon to 110 GPa Sample: at T = 300 K and P = 64.4 GPa
Hemley, R. J.; Zha, C. S.; Jephcoat, A. P.; Mao, H. K.; Finger, L. W.; Cox, D. E.; Physical Review B - Condensed Matter 39 (1989) 11820–11827; doi:10.1103/PhysRevB.39.11820

data_9011713
_publ_section_title
;
 X-ray diffraction and equation of state of solid neon to 110 GPa
 Sample: at T = 300 K and P = 64.4 GPa
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              11820
_journal_page_last               11827
_journal_paper_doi               10.1103/PhysRevB.39.11820
_journal_volume                  39
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ne
_chemical_name_common            Neon
_chemical_name_mineral           Neon
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_formula_units_Z            4
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.077
_cell_length_b                   3.077
_cell_length_c                   3.077
_cell_volume                     29.133
_database_code_amcsd             0015247
_diffrn_ambient_pressure         6.44e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.601
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9011713
X-ray diffraction and equation of state of solid neon to 110 GPa Sample: at T = 300 K and P = 74.3 GPa
Hemley, R. J.; Zha, C. S.; Jephcoat, A. P.; Mao, H. K.; Finger, L. W.; Cox, D. E.; Physical Review B - Condensed Matter 39 (1989) 11820–11827; doi:10.1103/PhysRevB.39.11820

data_9011714
_publ_section_title
;
 X-ray diffraction and equation of state of solid neon to 110 GPa
 Sample: at T = 300 K and P = 74.3 GPa
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              11820
_journal_page_last               11827
_journal_paper_doi               10.1103/PhysRevB.39.11820
_journal_volume                  39
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ne
_chemical_name_common            Neon
_chemical_name_mineral           Neon
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_formula_units_Z            4
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.035
_cell_length_b                   3.035
_cell_length_c                   3.035
_cell_volume                     27.956
_database_code_amcsd             0015248
_diffrn_ambient_pressure         7.43e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.795
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9011714
X-ray diffraction and equation of state of solid neon to 110 GPa Sample: at T = 300 K and P = 78.3 GPa
Hemley, R. J.; Zha, C. S.; Jephcoat, A. P.; Mao, H. K.; Finger, L. W.; Cox, D. E.; Physical Review B - Condensed Matter 39 (1989) 11820–11827; doi:10.1103/PhysRevB.39.11820

data_9011715
_publ_section_title
;
 X-ray diffraction and equation of state of solid neon to 110 GPa
 Sample: at T = 300 K and P = 78.3 GPa
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              11820
_journal_page_last               11827
_journal_paper_doi               10.1103/PhysRevB.39.11820
_journal_volume                  39
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ne
_chemical_name_common            Neon
_chemical_name_mineral           Neon
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_formula_units_Z            4
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.021
_cell_length_b                   3.021
_cell_length_c                   3.021
_cell_volume                     27.571
_database_code_amcsd             0015249
_diffrn_ambient_pressure         7.83e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.862
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9011715
X-ray diffraction and equation of state of solid neon to 110 GPa Sample: at T = 300 K and P = 82.3 GPa
Hemley, R. J.; Zha, C. S.; Jephcoat, A. P.; Mao, H. K.; Finger, L. W.; Cox, D. E.; Physical Review B - Condensed Matter 39 (1989) 11820–11827; doi:10.1103/PhysRevB.39.11820

data_9011716
_publ_section_title
;
 X-ray diffraction and equation of state of solid neon to 110 GPa
 Sample: at T = 300 K and P = 82.3 GPa
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              11820
_journal_page_last               11827
_journal_paper_doi               10.1103/PhysRevB.39.11820
_journal_volume                  39
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ne
_chemical_name_common            Neon
_chemical_name_mineral           Neon
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_formula_units_Z            4
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.014
_cell_length_b                   3.014
_cell_length_c                   3.014
_cell_volume                     27.380
_database_code_amcsd             0015250
_diffrn_ambient_pressure         8.23e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.895
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9011716
X-ray diffraction and equation of state of solid neon to 110 GPa Sample: at T = 300 K and P = 83.5 GPa
Hemley, R. J.; Zha, C. S.; Jephcoat, A. P.; Mao, H. K.; Finger, L. W.; Cox, D. E.; Physical Review B - Condensed Matter 39 (1989) 11820–11827; doi:10.1103/PhysRevB.39.11820

data_9011717
_publ_section_title
;
 X-ray diffraction and equation of state of solid neon to 110 GPa
 Sample: at T = 300 K and P = 83.5 GPa
;
_journal_name_full               'Physical Review B - Condensed Matter'
_journal_page_first              11820
_journal_page_last               11827
_journal_paper_doi               10.1103/PhysRevB.39.11820
_journal_volume                  39
_journal_year                    1989
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ne
_chemical_name_common            Neon
_chemical_name_mineral           Neon
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_formula_units_Z            4
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.003
_cell_length_b                   3.003
_cell_length_c                   3.003
_cell_volume                     27.081
_database_code_amcsd             0015251
_diffrn_ambient_pressure         8.35e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.949
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9011717